J Adv Prosthodont 2014;6:272-7
Evaluation of shear bond strength of repair acrylic resin to Co-Cr alloy Şafak Külünk1, Tolga Külünk1, Duygu Saraç1, Seda Cengiz2*, Seniha Baba1 1 2
Department of Prosthodontics, Faculty of Dentistry, 19 Mayis University, Samsun, Turkey Department of Prosthodontic, Faculty of Dentistry, Bülent Ecevit University, Zonguldak, Turkey
PURPOSE. The purpose of this study was to investigate the impact of different surface treatment methods and thermal ageing on the bond strength of autopolymerizing acrylic resin to Co-Cr. MATERIALS AND METHODS. Co-Cr alloy specimens were divided into five groups according to the surface conditioning methods. C: No treatment; SP: flamed with the Silano-Pen device; K: airborne particle abrasion with Al2O3; Co: airborne particle abrasion with silica-coated Al2O3; KSP: flamed with the Silano-Pen device after the group K experimental protocol. Then, autopolymerized acrylic resin was applied to the treated specimen surfaces. All the groups were divided into two subgroups with the thermal cycle and water storage to determine the durability of the bond. The bond strength test was applied in an universal test machine and treated Co-Cr alloys were analyzed by scanning electron microscope (SEM). Two-way analysis of variance (ANOVA) was used to determine the significant differences among surface treatments and thermocycling. Their interactons were followed by a multiple comparison' test performed uing a post hoc Tukey HSD test (α=.05). RESULTS. Surface treatments significantly increased repair strengths of repair resin to Co-Cr alloy. The repair strengths of Group K, and Co significantly decreased after 6,000 cycles (P.05). Significant differences among surface treatments and thermocycling was shown by two-way analysis of variance (ANOVA)(SPSS 12.0; SPSS Inc., Chicago, IL, USA). Their interactions were followed by a multiple comparisons’ test performed using a post hoc Tukey HSD test (α=.05).
RESULTS The means and standard deviations (SD) of the repair strengths after 0 and 6,000 cycles, along with the statistical comparisons of the groups are shown in Table 2. Two-way ANOVA indicated that surface treatment, thermo cycling and two-way interactions of surface treatment and thermo cycling were significantly different, and repair strength values varied according to the surface treatments and thermo cycling (P.05).
Table 3. The results of two-way ANOVA Source of variation
Sum of squares
Surface treatment * thermocycle
Evaluation of shear bond strength of repair acrylic resin to Co-Cr alloy
TC0 and TC1 groups except Group C, SP and KSP (P